The raw ore was ground to -200 mesh (71.5%) and treated through the flotation process of one-stage roughing, two-stage scavenging and three-stage concentration. Copper concentrates were treated by medium-intensity magnetic separator to remove pyrrhotite and other magnetic materials. The final copper concentrates had a yield of 5.25%, a Cu grade of 21% and a Cu recovery of 84.76%. The refused magnetic materials had an S grade of 31.86%, and were mixed with sulfur flotation concentrates as final sulfur concentrates. After slurry conditioning of tailings of copper flotation, the pH value was kept at around 6.5 and sodium sulfide was used to activate pyrite. Sulfur concentrates were produced through the common flotation process of one-stage roughing, one-stage scavenging and one-stage concentration, with a yield of 34.83%, an S grade of 58.5% and an S recovery of 82.26%. Tailings from sulfur flotation were treated in the magnetic separator to gain iron concentrates which had a yield of 8.67%, a Fe grade of 70.18% and an S grade of 1.63%.
An overflow ball mill with rolling bearings, high efficiency and energy saving.
JJF flotation cell is a air self-suction mechanical stirring floatation cell without slurry suction (Referring to the design of USA wemco flotation machine)
A mechanical agitation type floatation cell unit with air suction and combination of slurry suction/no slurry suction
Please write your message here! We will send detail technical info and quotation to you as soon as possible!